# A specimen of aluminum having a rectangular cross section 10 mm ```14:440:407 Ch6
Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm  12.7
mm (0.4 in.  0.5 in.) is pulled in tension with 35,500 N (8000 lbf) force, producing only
elastic deformation. Calculate the resulting strain.
Solution:
This problem calls for us to calculate the elastic strain that results for an aluminum specimen stressed in tension.
The cross-sectional area is just (10 mm)  (12.7 mm) = 127 mm2 (= 1.27  10-4 m2 = 0.20 in.2); also, the elastic
modulus for Al is given in Table 6.1 as 69 GPa (or 69  109 N/m2). Combining Equations 6.1 and 6.5 and solving
for the strain yields

F
35,500 N
=
=
= 4.1  10 -3
4
E
A0 E
(1.27  10 m2 )(69  10 9 N/m2 )
------------------------------------------------------------------------------------------------------------------------------------------- =
Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
(0.8 in.) on an edge is pulled in tension with a load of 89,000 N (20,000 lbf), and experiences
an elongation of 0.10 mm (4.0  10-3 in.). Assuming that the deformation is entirely elastic,
calculate the elastic modulus of the steel.
Solution:
This problem asks us to compute the elastic modulus of steel. For a square cross-section, A0 = b02 , where
b0 is the edge length. Combining Equations 6.1, 6.2, and 6.5 and solving for E, leads to
F
Fl

A0
=
= 20
E =
l

b0 l
l0
=
(89,000 N) (100  103 m)
(20  103 m) 2 ( 0.10  103 m)
= 223  109 N/m2 = 223 GPa (31.3  106 psi)
Question 6.7: For a bronze alloy, the stress at which plastic deformation begins is 275 MPa
(40,000 psi), and the modulus of elasticity is 115 GPa (16.7  106 psi).
(a) What is the maximum load that may be applied to a specimen with a cross-sectional
area of 325 mm2 (0.5 in.2) without plastic deformation?
(b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to
which it may be stretched without causing plastic deformation?
Solution:
(a) This portion of the problem calls for a determination of the maximum load that can be applied without
plastic deformation (Fy). Taking the yield strength to be 275 MPa, and employment of Equation 6.1 leads to
Fy =  y A0 = (275  10 6 N/m 2 )(325  10 -6 m 2 )
= 89,375 N (20,000 lbf)
(b) The maximum length to which the sample may be deformed without plastic deformation is determined
from Equations 6.2 and 6.5 as

 
li = l0 1  

E 

275 MPa 
= (115 mm) 1 
= 115.28 mm (4.51 in.)
 115  10 3 MPa 
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.13: In Section 2.6 it was noted that the net bonding energy EN between two
isolated positive and negative ions is a function of interionic distance r as follows:
EN  
A B

r rn
(6.25)
where A, B, and n are constants for the particular ion pair. Equation 6.25 is also valid for
the bonding energy between adjacent ions in solid materials. The modulus of elasticity E is
proportional to the slope of the interionic force–separation curve at the equilibrium
interionic separation; that is,
dF 
E   
dr r
o
Derive an expression for the dependence of the modulus of elasticity on these A, B, and n
parameters (for the two-ion system) using the following procedure:
1. Establish a relationship for the force F as a function of r, realizing that
F
dEN
dr
2. Now take the derivative dF/dr.
3. Develop an expression for r0, the equilibrium separation. Since r0 corresponds to
the value of r at the minimum of the EN-versus-r curve (Figure 2.8b), take the derivative
dEN/dr, set it equal to zero, and solve for r, which corresponds to r0.
4. Finally, substitute this expression for r0 into the relationship obtained by taking
dF/dr.
Solution:
This problem asks that we derive an expression for the dependence of the modulus of elasticity, E, on the
parameters A, B, and n in Equation 6.25. It is first necessary to take dEN/dr in order to obtain an expression for the
force F; this is accomplished as follows:
 B 
 A 
d   d n 
dE N
 r 
r 
=
+
F =
dr
dr
dr
=
A
r2

nB
r (n 1)
The second step is to set this dEN/dr expression equal to zero and then solve for r (= r0). The algebra for this
procedure is carried out in Problem 2.14, with the result that
 A 1/(1  n)
r0 =  
nB 
Next it becomes necessary to take the derivative of the force (dF/dr), which is accomplished as follows:
 A 
 nB 
d   d 

2
dF
r 
 r (n 1) 
=
+
dr
dr
dr
=
2A
r3
+
(n)(n  1) B
r (n  2)
Now, substitution of the above expression for r0 into this equation yields
dF 
2A
(n)(n  1) B
+
  = 
3/(1
n)
dr r
 A 
 A (n  2) /(1 n)
0
 
 
nB 
nB 
which is the expression to which the modulus of elasticity is proportional.
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.14: Using the solution to Problem 6.13, rank the magnitudes of the moduli of
elasticity for the following hypothetical X, Y, and Z materials from the greatest to the least.
The appropriate A, B, and n parameters (Equation 6.25) for these three materials are
tabulated below; they yield EN in units of electron volts and r in nanometers:
Material
A
B
n
X
Y
Z
2.5
2.3
3.0
2.0 &times; 10–5
8.0 &times; 10–6
1.5 &times; 10–5
8
10.5
9
Solution:
This problem asks that we rank the magnitudes of the moduli of elasticity of the three hypothetical metals
X, Y, and Z. From Problem 6.13, it was shown for materials in which the bonding energy is dependent on the
interatomic distance r according to Equation 6.25, that the modulus of elasticity E is proportional to
E 
2A
3/(1 n)
 A
 
nB 
+
(n)(n  1) B
 A (n  2) /(1 n)
 
nB 
For metal X, A = 2.5, B = 2.0  10-5, and n = 8. Therefore,
E  
(2)(2.5)


(8)

3/(1  8)
2.5

2  105 

(
(8)(8  1) (2  105 )
+

(8  2) /(1  8)
2.5


(8) (2  105 ) 
)
= 1097
For metal Y, A = 2.3, B = 8  10-6, and n = 10.5. Hence
E  
(2)(2.3)


(10.5)

2.3
(8 
3/(1  10.5)

106 

+
)
(10.5)(10.5  1) (8  106 )

(10.5  2) /(1  10.5)
2.3


(10.5) (8  106 ) 
= 551
And, for metal Z, A = 3.0, B = 1.5  10-5, and n = 9. Thus
E  
(2)(3.0)


(9)

3/(1  9)

3.0

5
(1.5  10 ) 
+
(9)(9  1) (1.5  105 )

(9  2) /(1  9)
3.0


(9) (1.5  105 ) 
= 1024
Therefore, metal X has the highest modulus of elasticity.
--------------------------------------------------------------------------------------------------------------------------------------------
Question 15: A cylindrical specimen of aluminum having a diameter of 19 mm (0.75 in.)
and length of 200 mm (8.0 in.) is deformed elastically in tension with a force of 48,800 N
(11,000 lbf). Using the data contained in Table 6.1, determine the following:
(a) The amount by which this specimen will elongate in the direction of the applied stress.
(b) The change in diameter of the specimen. Will the diameter increase or decrease?
Solution:
(a) We are asked, in this portion of the problem, to determine the elongation of a cylindrical specimen of
aluminum. Combining Equations 6.1, 6.2, and 6.5, leads to
 = E
F
l
=E
d 2 
l0
  0 
 4 
 
Or, solving for l (and realizing that E = 69 GPa, Table 6.1), yields
l =
=
4 F l0
 d02 E
(4)(48,800 N) (200  103 m)
 5  10 -4 m = 0.50 mm (0.02 in.)
() (19  103 m)2 (69  10 9 N / m2 )
(b) We are now called upon to determine the change in diameter, d. Using Equation 6.8

d / d0
 =  x = 
z
 l / l0
From Table 6.1, for aluminum,  = 0.33. Now, solving the above expression for ∆d yields
d = 
 l d0
(0.33)(0.50 mm)(19 mm)
= 
200 mm
l0
= –1.6  10-2 mm (–6.2  10-4 in.)
The diameter will decrease.
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.20: A brass alloy is known to have a yield strength of 275 MPa (40,000 psi), a
tensile strength of 380 MPa (55,000 psi), and an elastic modulus of 103 GPa (15.0  106 psi).
A cylindrical specimen of this alloy 12.7 mm (0.50 in.) in diameter and 250 mm (10.0 in.)
long is stressed in tension and found to elongate 7.6 mm (0.30 in.). On the basis of the
information given, is it possible to compute the magnitude of the load that is necessary to
produce this change in length? If so, calculate the load. If not, explain why.
Solution:
We are asked to ascertain whether or not it is possible to compute, for brass, the magnitude of the load necessary to
produce an elongation of 7.6 mm (0.30 in.). It is first necessary to compute the strain at yielding from the yield
strength and the elastic modulus, and then the strain experienced by the test specimen. Then, if
(test) &lt; (yield)
deformation is elastic, and the load may be computed using Equations 6.1 and 6.5. However, if
(test) &gt; (yield)
computation of the load is not possible inasmuch as deformation is plastic and we have neither a stress-strain plot
nor a mathematical expression relating plastic stress and strain. We compute these two strain values as
(test) =
and
(yield) =
y
E
l
7.6 mm
=
= 0.03
l0
250 mm
=
275 MPa
= 0.0027
103  10 3 MPa
Therefore, computation of the load is not possible since (test) &gt; (yield).
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.22: Consider the brass alloy for which the stress-strain behavior is shown in
Figure 6.12. A cylindrical specimen of this material 6 mm (0.24 in.) in diameter and 50 mm
(2 in.) long is pulled in tension with a force of 5000 N (1125 lbf). If it is known that this
alloy has a Poisson's ratio of 0.30, compute: (a) the specimen elongation, and (b) the
reduction in specimen diameter.
Solution:
(a) This portion of the problem asks that we compute the elongation of the brass specimen. The first
calculation necessary is that of the applied stress using Equation 6.1, as
 =
F
=
A0
F
2
d 
  0 
 2 
=
5000 N
6  103 m 2
 

2


= 177  10 6 N/m2 = 177 MPa (25,000 psi)
From the stress-strain plot in Figure 6.12, this stress corresponds to a strain of about 2.0  10-3. From the definition
of strain, Equation 6.2
l = l0 = (2.0  10 -3) (50 mm) = 0.10 mm (4  10 -3 in.)
(b) In order to determine the reduction in diameter ∆d, it is necessary to use Equation 6.8 and the definition
of lateral strain (i.e., x = ∆d/d0) as follows
d = d0x =  d0   z =  (6 mm)(0.30) (2.0  10 -3)
= –3.6  10-3 mm (–1.4  10-4 in.)
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.27: A load of 85,000 N (19,100 lbf) is applied to a cylindrical specimen of a steel
alloy (displaying the stress–strain behavior shown in Figure 6.21) that has a cross-sectional
diameter of 15 mm (0.59 in.).
(a) Will the specimen experience elastic and/or plastic deformation? Why?
(b) If the original specimen length is 250 mm (10 in.), how much will it increase in length
Solution:
This problem asks us to determine the deformation characteristics of a steel specimen, the stress-strain
behavior for which is shown in Figure 6.21.
(a) In order to ascertain whether the deformation is elastic or plastic, we must first compute the stress, then
locate it on the stress-strain curve, and, finally, note whether this point is on the elastic or plastic region. Thus, from
Equation 6.1
 =
F
=
A0
85,000 N
15  103 m 2
 

2


= 481  10 6 N/m2 = 481 MPa (69, 900 psi)
The 481 MPa point is beyond the linear portion of the curve, and, therefore, the deformation will be both elastic and
plastic.
(b) This portion of the problem asks us to compute the increase in specimen length. From the stress-strain
curve, the strain at 481 MPa is approximately 0.0135. Thus, from Equation 6.2
l =  l0 = (0.0135)(250 mm) = 3.4 mm (0.135 in.)
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.28: A bar of a steel alloy that exhibits the stress-strain behavior shown in Figure
6.21 is subjected to a tensile load; the specimen is 300 mm (12 in.) long, and of square cross
section 4.5 mm (0.175 in.) on a side.
(a) Compute the magnitude of the load necessary to produce an elongation of 0.45 mm
(0.018 in.).
(b) What will be the deformation after the load has been released?
Solution:
(a) We are asked to compute the magnitude of the load necessary to produce an elongation of 0.45 mm for
the steel displaying the stress-strain behavior shown in Figure 6.21. First, calculate the strain, and then the
corresponding stress from the plot.
 =
l 0.45 mm
=
=1.5  103
l0
300 mm
This is near the end of the elastic region; from the inset of Figure 6.21, this corresponds to a stress of about 300
MPa (43,500 psi). Now, from Equation 6.1
F = A0 = b 2
in which b is the cross-section side length. Thus,
F = (300  10 6 N/m2 ) (4.5  10 -3 m) 2 = 6075 N (1366 lb f )
(b) After the load is released there will be no deformation since the material was strained only elastically.
Question 6.29: A cylindrical specimen of aluminum having a diameter of 0.505 in. (12.8
mm) and a gauge length of 2.000 in. (50.800 mm) is pulled in tension. Use the load–
elongation characteristics tabulated below to complete parts (a) through (f).
Length
N
lbf
mm
in.
0
0
50.800
2.000
7,330
1,650
50.851
2.002
15,100
3,400
50.902
2.004
23,100
5,200
50.952
2.006
30,400
6,850
51.003
2.008
34,400
7,750
51.054
2.010
38,400
8,650
51.308
2.020
41,300
9,300
51.816
2.040
44,800
10,100
52.832
2.080
46,200
10,400
53.848
2.120
47,300
10,650
54.864
2.160
47,500
10,700
55.880
2.200
46,100
10,400
56.896
2.240
44,800
10,100
57.658
2.270
42,600
9,600
58.420
2.300
36,400
8,200
59.182
2.330
Fracture
(a) Plot the data as engineering stress versus engineering strain.
(b) Compute the modulus of elasticity.
(c) Determine the yield strength at a strain offset of 0.002.
(d) Determine the tensile strength of this alloy.
(e) What is the approximate ductility, in percent elongation?
(f) Compute the modulus of resilience.
Solution:
This problem calls for us to make a stress-strain plot for aluminum, given its tensile load-length data, and
then to determine some of its mechanical characteristics.
(a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve, while for
the second, the curve extends to just beyond the elastic region of deformation.
(b) The elastic modulus is the slope in the linear elastic region (Equation 6.10) as
E =
  200 MPa  0 MPa
=
= 62.5  10 3 MPa = 62.5 GPa (9.1  10 6 psi)
0.0032  0

(c) For the yield strength, the 0.002 strain offset line is drawn dashed. It intersects the stress-strain curve at
approximately 285 MPa (41,000 psi ).
(d) The tensile strength is approximately 370 MPa (54,000 psi), corresponding to the maximum stress on
the complete stress-strain plot.
(e) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-hundred. The
total fracture strain at fracture is 0.165; subtracting out the elastic strain (which is about 0.005) leaves a plastic
strain of 0.160. Thus, the ductility is about 16%EL.
(f) From Equation 6.14, the modulus of resilience is just
Ur =
 2y
2E
which, using data computed above gives a value of
Ur =
(285 MPa) 2
= 0.65 MN/m2  0.65  10 6 N/m2  6.5  10 5 J/m3
(2) (62.5  10 3 MPa)
(93.8
in.- lb f /in.3)
--------------------------------------------------------------------------------------------------------------------Question 6.40: Demonstrate that Equation 6.16, the expression defining true strain, may
also be represented by
A 
Ai 
∈T = ln  0 
when specimen volume remains constant during deformation. Which of these two
expressions is more valid during necking? Why?
Solution:
This problem asks us to demonstrate that true strain may also be represented by
A 
∈T = ln  0 
Ai 
Rearrangement of Equation 6.17 leads to
li
l0
=
A0
Ai
Thus, Equation 6.16 takes the form
l 
A 
∈T = ln  i  = ln  0 
l0 
 Ai 
A 
The expression ∈T = ln  0  is more valid during necking because Ai is taken as the area of the neck.
Ai 
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.44: The following true stresses produce the corresponding true plastic strains
for a brass alloy:
True Stress (psi)
True Strain
50,000
60,000
0.10
0.20
What true stress is necessary to produce a true plastic strain of 0.25?
Solution:
For this problem, we are given two values of T and T, from which we are asked to calculate the true
stress which produces a true plastic strain of 0.25. Employing Equation 6.19, we may set up two simultaneous
equations with two unknowns (the unknowns being K and n), as
log (50,000 psi) = log K + n log (0.10)
log (60,000 psi) = log K + n log (0.20)
Solving for n from these two expressions yields
n=
and for K
log (50,000)  log (60, 000)
= 0.263
log (0.10)  log (0.20)
log K = 4.96 or K = 104.96 = 91,623 psi
Thus, for T = 0.25
 T = K (T ) n = (91,623 psi)(0.25)0.263 = 63,700 psi (440 MPa)
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.46: Find the toughness (or energy to cause fracture) for a metal that experiences
both elastic and plastic deformation. Assume Equation 6.5 for elastic deformation, that the
modulus of elasticity is 172 GPa (25  106 psi), and that elastic deformation terminates at a
strain of 0.01. For plastic deformation, assume that the relationship between stress and
strain is described by Equation 6.19, in which the values for K and n are 6900 MPa (1  106
psi) and 0.30, respectively. Furthermore, plastic deformation occurs between strain values
of 0.01 and 0.75, at which point fracture occurs.
Solution:
This problem calls for us to compute the toughness (or energy to cause fracture). The easiest way to do this
is to integrate both elastic and plastic regions, and then add them together.
Toughness =   d
0.01
=
 E d 
0
=
=
E2
2
 Kn d 
0.01
0.01
+
0
0.75
+
K
( n  1)
(n  1)
0.75
0.01
172  10 9 N/m2
6900  10 6 N/ m2
(0.01) 2 +
(0.75)1.3  (0.01) 1.3
2
(1.0  0.3)


= 3.65  109 J/m3 (5.29  105 in.-lbf/in.3)
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.49: A cylindrical specimen of a brass alloy 7.5 mm (0.30 in.) in diameter and
90.0 mm (3.54 in.) long is pulled in tension with a force of 6000 N (1350 lbf); the force is
subsequently released.
(a) Compute the final length of the specimen at this time. The tensile stress–strain behavior
for this alloy is shown in Figure 6.12.
(b) Compute the final specimen length when the load is increased to 16,500 N (3700 lbf) and
then released.
Solution:
(a) In order to determine the final length of the brass specimen when the load is released, it first becomes
necessary to compute the applied stress using Equation 6.1; thus
 =
F
=
A0
F
d 2
 0 
 2 
=
6000 N
7.5  103 m 2


2


= 136 MPa (19, 000 psi)
Upon locating this point on the stress-strain curve (Figure 6.12), we note that it is in the linear, elastic region;
therefore, when the load is released the specimen will return to its original length of 90 mm (3.54 in.).
(b) In this portion of the problem we are asked to calculate the final length, after load release, when the
load is increased to 16,500 N (3700 lbf). Again, computing the stress
 =
16, 500 N
7.5  103 m 2
 

2


= 373 MPa (52, 300 psi)
The point on the stress-strain curve corresponding to this stress is in the plastic region. We are able to estimate the
amount of permanent strain by drawing a straight line parallel to the linear elastic region; this line intersects the
strain axis at a strain of about 0.08 which is the amount of plastic strain. The final specimen length li may be
determined from a rearranged form of Equation 6.2 as
li = l0(1 + ) = (90 mm)(1 + 0.08) = 97.20 mm (3.82 in.)
--------------------------------------------------------------------------------------------------------------------------------------------
Question 6.D1: A large tower is to be supported by a series of steel wires. It is estimated
that the load on each wire will be 11,100 N (2500 lbf). Determine the minimum required
wire diameter assuming a factor of safety of 2 and a yield strength of 1030 MPa (150,000
psi).
Solution:
For this problem the working stress is computed using Equation 6.24 with N = 2, as
w =
y
2
=
1030 MPa
= 515 MPa (75, 000 psi )
2
Since the force is given, the area may be determined from Equation 6.1, and subsequently the original diameter d0
may be calculated as
A0 =
d 2
F
=   0 
w
 2 
And
d0 =
4F
=
 w
(4)(11,100 N)
 (515  10 6 N / m 2 )
= 5.23  10-3 m = 5.23 mm (0.206 in.)
--------------------------------------------------------------------------------------------------------------------Question 6.D2: (a) Gaseous hydrogen at a constant pressure of 1.013 MPa (10 atm) is to
flow within the inside of a thin-walled cylindrical tube of nickel that has a radius of 0.1 m.
The temperature of the tube is to be 300C and the pressure of hydrogen outside of the
tube will be maintained at 0.01013 MPa (0.1 atm). Calculate the minimum wall thickness if
the diffusion flux is to be no greater than 1  10-7 mol/m2-s. The concentration of hydrogen
in the nickel, CH (in moles hydrogen per m3 of Ni) is a function of hydrogen pressure, PH2
(in MPa) and absolute temperature (T) according to
 12.3 kJ/mol 
CH  30.8 pH 2 exp



RT
(6.28)
Furthermore, the diffusion coefficient for the diffusion of H in Ni depends on temperature
as
 39.56 kJ/mol 
DH  4.76  107 exp



RT
(6.29)
(b) For thin-walled cylindrical tubes that are pressurized, the circumferential stress
is a function of the pressure difference across the wall (Δp), cylinder radius (r), and tube
thickness (Δx) as
 =
r p
4 x
(6.30)
Compute the circumferential stress to which the walls of this pressurized cylinder are
exposed.
(c) The room-temperature yield strength of Ni is 100 MPa (15,000 psi) and,
furthermore, sy diminishes about 5 MPa for every 50C rise in temperature. Would you
expect the wall thickness computed in part (b) to be suitable for this Ni cylinder at 300C?
Why or why not?
(d) If this thickness is found to be suitable, compute the minimum thickness that
could be used without any deformation of the tube walls. How much would the diffusion
flux increase with this reduction in thickness? On the other hand, if the thickness
determined in part (c) is found to be unsuitable, then specify a minimum thickness that you
would use. In this case, how much of a diminishment in diffusion flux would result?
Solution:
(a) This portion of the problem asks for us to compute the wall thickness of a thin-walled cylindrical Ni
tube at 300C through which hydrogen gas diffuses. The inside and outside pressures are, respectively, 1.1013 and
0.01013 MPa, and the diffusion flux is to be no greater than 1  10-7 mol/m2-s. This is a steady-state diffusion
problem, which necessitates that we employ Equation 5.3. The concentrations at the inside and outside wall faces
may be determined using Equation 6.28, and, furthermore, the diffusion coefficient is computed using Equation
6.29. Solving for x (using Equation 5.3)
x = 
= 
(4.76 
1 
107
D C
J
1

mol/m2  s


39, 560 J / mol
10 -7 ) exp 
 
 (8.31 J/mol- K)(300  273 K) 


12,300 J/mol
(30.8) exp

 (8.31 J/mol- K)(300  273 K) 

0.01013 MPa 
1.1013 MPa

= 0.0025 m = 2.5 mm
(b) Now we are asked to determine the circumferential stress:
 =
=
r p
4 x
(0.10 m)(1.013 MPa  0.01013 MPa)
(4)(0.0025 m)
= 10.0 MPa
(c) Now we are to compare this value of stress to the yield strength of Ni at 300C, from which it is
possible to determine whether or not the 2.5 mm wall thickness is suitable. From the information given in the
problem, we may write an equation for the dependence of yield strength (y) on temperature (T) as follows:
 y = 100 MPa 
5 MPa
T  Tr
50C


where Tr is room temperature and for temperature in degrees Celsius. Thus, at 300C
 y = 100 MPa  (0.1 MPa/C) (300C  20C) = 72 MPa
Inasmuch as the circumferential stress (10 MPa) is much less than the yield strength (72 MPa), this thickness is
entirely suitable.
(d) And, finally, this part of the problem asks that we specify how much this thickness may be reduced and
still retain a safe design. Let us use a working stress by dividing the yield stress by a factor of safety, according to
Equation 6.24. On the basis of our experience, let us use a value of 2.0 for N. Thus
w =
y
N
=
72 MPa
= 36 MPa
2
Using this value for w and Equation 6.30, we now compute the tube thickness as
x =

r p
4w
(0.10 m)(1.013 MPa  0.01013 MPa)
4(36 MPa)
= 0.00070 m = 0.70 mm
Substitution of this value into Fick's first law we calculate the diffusion flux as follows:
J = D
C
x


39,560 J/mol
=  (4.76  10 -7 ) exp 
 
 (8.31 J/mol- K)(300  273 K) 


12, 300 J / mol
(30.8) exp 
 0.01013 MPa 
 (8.31 J/mol - K)(300  273 K) 
0.0007 m

1.013 MPa

= 3.53  10-7 mol/m2-s
Thus, the flux increases by approximately a factor of 3.5, from 1  10-7 to 3.53  10-7 mol/m2-s with this reduction
in thickness.
--------------------------------------------------------------------------------------------------------------------------------------------
```